CHAPTER 4 MACROMECHANICAL ANALYSIS OF LAMINATES. Dr. Ahmet Erkliğ. Laminate Code. A laminate is made of a group of single layers bonded to each other. Each layer can be identiﬁed by its location in the laminate, its material, and its angle of orientation with a reference axis.
Dr. Ahmet Erkliğ
A laminate is made of a group of single layers bonded to each other.
Eachlayer can be identiﬁed by its location in the laminate, its material, and itsangle of orientation with a reference axis.
subscript s outside the brackets represents that the three plies are repeated in the reverse order.
T stands for a total laminate.
The classical lamination theory is used to develop these relationships.Assumptions:
Nx = normal force resultant in the x direction (per unit length)
Ny = normal force resultant in the y direction (per unit length)
Nxy = shear force resultant (per unit length)
Mx = bending moment resultant in the yz plane (per unit length)
My = bending moment resultant in the xz plane (per unit length)
Mxy = twisting moment resultant (per unit length)
Curvatures in the laminate
Distance from the midplane in the thickness direction
Midplane strains in the laminate
Consider a laminate made of n plies. Each ply has athickness of tk. Then the thickness of the laminate h is
The z-coordinate of each ply k surface (top and bottom) isgiven by
Ply k: (k = 2, 3,…n – 2, n – 1):
Integrating the global stresses in each lamina gives the resultant forces perunit length in the x–y plane through the laminate thickness as
Similarly, integrating the global stresses in each lamina gives the resulting moments per unit length in the x–y plane through the laminate thickness as
The midplane strains and platecurvatures are independent of the z-coordinate. Also, the transformedreduced stiffness matrixis constant for each ply.
[A] – extensional stiffness matrix relating the resultant in-plane forces to the in-plane strains.
[B] – coupling stiffness matrix coupling the force and moment terms to the midplane strains and midplane curvatures.
[D] – bending stiffness matrix relating the resultant bending moments to the plate curvatures.
Find the three stiffness matrices [A], [B], and [D] for a three-ply [0/30/-45]graphite/epoxy laminate as shown in Figure. Assume that each lamina hasa thickness of 5 mm.
Step 1: Find the reduced stiffness matrix [Q] for each ply
Step 2: Find the transformed stiffness matrix  using the reduced stiffness matrix [Q] and the angle of the ply
Step 3: Find the coordinate of the top and bottom surface of each plyusingequation 4.20
The total thickness of the laminate is h = (0.005)(3) = 0.015 m.
The midplane is 0.0075 m from the top and the bottom of the laminate.
h0 = –0.0075 m
h1 = –0.0025 m
h2 = 0.0025 m
h3 = 0.0075 m
A [0/30/–45] graphite/epoxy laminate is subjected to a load of Nx = Ny =1000 N/m.Find,
The strains and stresses at the top surface of the 30° ply are foundas follows. First, the top surface of the 30° ply is located at z = h1 =–0.0025 m.